Università degli Studi di Cagliari
DOTTORATO DI RICERCA
Scienze e Tecnologie Chimiche
DESIGN OF FUNCTIONAL COLLOIDAL MAGNETIC
NANOPARTICLES FOR BIOMEDICAL APPLICATIONS
Settore/i scientifico disciplinari di afferenza
Presentata da: Dott.ssa Federica Orrù
Coordinatore Dottorato: Prof. Mariano Casu
Relatore: Dott.ssa Carla Cannas
A Science has great beauty. A scientist in his laboratory is not only a technician: he is also a child placed before natural phenomena which impress him like a fairy tale. ( Marie Curie)
Nanostructured materials have been the focus of scientific interest in recent years, because of the peculiar properties displayed by matter in nano-size form. The interest has been growing steeply since possible applications in biomedical fields have shown to be realistic. The interaction of magnetic nanoparticles with applied magnetic field gradients makes these particles attractive for their potential applications in biomedical
imaging, diagnostic, and therapy. In this context, a great advantage are the
superparamagnetic properties that can be exhibited by the nanoparticles. They behave as paramagnetic centres with high magnetic moment at room temperature, as it arises from the coupling of many atomic spins. After eliminating the external magnetic field, the particles no longer show magnetic interaction, thus reducing the possibility of particle aggregation; this feature is especially important for their applications. Biomedical use of magnetic nanoparticles imposes their uniform dispersion and stability in the biological fluids; moreover their size range should easily permit cell internalization through pinocytosis or endocytosis. Therefore, surface modification, via coating or encapsulation, is widely employed to improve nanoparticles properties and for immobilization of functional molecules. Magnetic nanoparticles have garnered widespread attention in recent years to develop and understand synthetic means to control their size, magnetic behaviour, and chemical reactivity. Simultaneously tuning surface chemistry and physical properties enable preparation of functional magnetic nanoparticles. Recent advances in synthesis have allowed to easily prepare a wide range of magnetic nanoparticles though aqueous or non aqueous approaches. It has been widely shown that the non-aqueous routes are more efficient in producing stable colloidal nanoparticles with narrow size distribution, high crystallinity, tunable size and shape. However, this approach typically produces hydrophobic nanoparticles limiting their applications in biological and medical fields. Thus, the transformation of these
hydrophobic nanoparticles into hydrophilic is a crucial step toward their widespread use.
The aim of the present PhD research project is to give a contribution to implement synthetic approaches to develop novel colloidal magnetic nano-architectures with applications in biomedical field. In particular, the research moves along two principal themes. From one side it has been investigated the possibility to tune magnetic nanoparticles size and properties through appropriate synthetic methodologies. From the other side, since the selected synthetic approach provides hydrophobic nanoparticles, particular attention has been devoted to the surface modification with organic and inorganic coatings in order to convert them into water dispersible systems. To this end, a multi-technique approach is used. A first structural analysis is performed by wide-angle X-ray Diffraction to obtain information about the crystalline phases and the crystallite size (coherent domain). Direct images of the samples, obtained by Transmission Electron Microscopy observations allowed an evaluation of the particle sizes, their distribution and the homogeneity of the particle dispersions.
In order to study the magnetic-nanoparticles/coating interface, studies with FT-IR spectroscopy have been performed on hydrophobic nanoparticles and on all the systems in which the surface modification has been applied. To investigate the textural properties of the silica based composites nitrogen physisorption measurements have been performed in combination with low-angle X-ray diffraction to evidence the ordered porosity. Magnetic measurements have been acquired in order to understand how the different chemical composition, size and coatings can affect the magnetic properties of nanoparticles.
All the measurements have been carried out at the Department of Chemical and Geological Sciences at the University of Cagliari.
The present thesis is structured as follow: after an introduction on magnetic nanoparticle applications and properties (chapter 1), the chapter 2 is devoted to the magnetic nanoparticles with a special emphasis on the different surface chemical
modification processes for their transferring into water environment. In the chapter 3 a synthetic approach based on a surfactant-assisted high-temperature thermal decomposition of metallorganic compounds is described in order to prepare hydrophobic magnetite and cobalt ferrite nanoparticles with different sizes, narrow particle size distributions and tuned magnetic properties. Magnetite is an ideal candidate material because of its documented biocompatibility and high saturation magnetization, cobalt ferrite has been also chosen because of its known large magnetic
anisotropy compared to other ferrites, in spite of highly toxic cobalt. In the chapter 4
magnetic nanoparticles possessing a hydrophobic surface are transferred into water through molecular coatings. Oleic acid/oleylamine molecules, bound to the surface of magnetic nanoparticles, are substituted (ligand–exchange) by molecules possessing a dual functionality that allows their dispersion in water. The selected molecules are short-chain dicarboxylic acids or alkylsilanes. These molecules form a coating on the surface of the magnetic nanoparticles via carboxylic or Me-O-Si bonds, ensuring their stability in aqueous environment, as well as creating the conditions for a their possible conjugation with biologically active molecules. The hydrophobic nanoparticles is converted into hydrophilic also through the intercalation process with suitable
surfactants such as cetyltrimethylammonium bromide (CTAB). These “magnetic pseudo
micelles” build up of an inorganic core (magnetite or cobalt ferrite) and an organic shell
(oleic acid-oleylamine-CTAB) are stable in water and can be employed in biological
field. In the chapter 5 pure CTAB micelles are also used as organic templates for the
formation of colloidal mesostructured silica nanoparticles through a base-catalyzed sol-gel process. The hybrid-organic-inorganic “magnetic pseudo micelles”, have been proposed as
building blocks for the creation, through the self assembling processes, of colloidal magnetic mesostructured silica nanoparticles with hexagonal or cubic pore structure. Silica is stable, biocompatible and hydrophilic, and if prepared in the form of mesostructured nanoparticles, showing high surface area and high pore volume, allows to incorporate an high number of magnetic nanoparticles, and to associate to the
magnetic properties other properties by entrapping fluorescent molecules, quantum dots, or luminescent nanoparticles.
Due to their peculiar features, these colloidal magnetic nanocarriers can be considered promising versatile multifunctional systems for applications in theranostic as well as in bimodal (magnetic and optic) imaging applications. For these reasons, at
last, some general commentsand future insights are given.
IndexForeword……….. ... i-iv
Chapter 1. Magnetic Metal Oxide Nanoparticles in Biomedical Applications…..
1.0 Magnetic Metal Oxide Nanoparticles and Biomedical Applications ... 2
1.1 Introduction ... 2
1.2 Superparamagnetic Nanoparticles ... 4
1.3 Synthesis Techniques: Iron Oxide Nanoparticles ... 7
1.4 Biomedical applications of Magnetic Nanoparticles ... 9
1.4.1 Therapeutic applications ... 10
1.4.2 Diagnostic applications ... 15
References ... 22
Chapter2. Magnetic Nanoparticles: Surface Modification and Silica Nanocomposite . ... 27-43 2.0 Surface modification of magnetic nanoparticles ... 28
2.1 Introduction ... 28
2.2 Surface modification ... 29
2.2.1 Organic coating ... 30
2.2.2 Mechanisms of surface modification by organic molecules ... 31
2.2.3 Inorganic coating... 33
2.2.4 Silica coating ... 34
vi Chapter 3. Colloidal Magnetic Nanoparticles prepared by high temperature
thermal decomposition of organometallic precursors assisted by surfactants(HTDSA)………44-71
3.0 Experimental ... 45
3.1 Introduction ... 45
3.2 Nucleation and growth mechanism in HTDSA strategy ... 46
3.3 Synthesis of Spinel Ferrite Nanoparticles ... 50
3.3.1 CoFe2O4 nanoparticles: Characterization ...52
3.3.2 Fe3O4 nanoparticles: Characterization ... 61
3.4 Conclusions ... 67
References ... 69
Chapter 4. Trasferring of hydrophobic nanoparticles into water: Legend exchange and Intercalation processes . ... 72-98 4.0 Experimental ... 73
4.1 Introduction ... 73
4.2 Legend Exchange with carboxylic acid and alkylsilane ... 73
4.2.1 Ligand Exchange with short chain carboxylic acids ... 75
4.2.2 Characterization ... 76
4.3 Ligand Exchange with alkylsilane ... 83
4.3.1 Ligand Exchange with alkylsilanes ...86
4.3.2 Characterization ... 87
4.4 Intercalation process with CTAB (MAG_CTAB) ... 91
4.4.1 Characterization ... 93
4.5 Conclusions ... 95
vii Chapter 5. Colloidal Magnetic Mesostructured Silica Nanoparticles . ... 99-141
5.0 Experimental ... 100
5.1 Introduction ... 100
5.2 Mesoporous Silica Nanoparticles ... 105
5.3 Hexagonal and Cubic Mesostructured Silica nanoparticles (MSN_H, MSN_C): synthesis and characterization ... 108
5.3.1 Synthesis ... 108
5.3.2 Microstructural and textural Characterization ... 112
5.4 Magnetic mesostructured silica based nanoparticles (MMSN_H and MMSN_C): Synthesis, characterization and magnetic properties ... 121
5.4.1 Introduction ... 121
5.4.2 MMSN_H Synthesis ... 123
5.4.3 Characterization ... 125
5.5 Conclusions ...138
References ... 139
Conclusions and future insights. ... 142-145 Appendix Equipments and Techniques. ... 146-151 Acknowledgements. ... 152
Magnetic Metal Oxide Nanoparticles
in Biomedical Applications
This chapter gives general information about properties of magnetic nanomaterials, synthesis approaches and biomedical applications. It provides the background for understanding and exploring the biomedical applications of magnetic nanoparticles.
Magnetic Metal Oxide Nanoparticles
in Biomedical Applications
1.0 Magnetic Metal Oxide Nanoparticles and Biomedical Applications 1.1 Introduction
The development of novel materials is a fundamental focal point of chemical research; and this interest is mandated by advancements in all areas of industry and technology. Therefore in the last decade, the scientific research has focused on the development of new materials at the atomic, molecular, or macromolecular levels, on the length scale of approximately 1-100 nm. These research efforts are expected to provide a fundamental understanding of phenomena and materials at the nanoscale and to create and use structures, devices, and systems that have novel properties and functions due to their
small and/or intermediate size, typically under 100 nm. Successful application of
nanoparticles not only depends on the special properties exhibited at this scale such as an enhanced electronic, mechanical, and chemical response but also on their manipulation to achieve specific objectives. In this sense, magnetic nanoparticles offer a range of opportunities as their response can be tailored by choosing from a variety of magnetic materials with different magnetic properties that can be manipulated by the use of external magnetic fields and by modification of their surfaces with molecules specific for intended applications.
Magnetic nanoparticles are a major class of nanoscale materials with the potential to revolutionize current clinical diagnostic and therapeutic techniques. Due to their unique physical properties and ability to function at the cellular and molecular
level of biological interactions, they are being actively investigated as the next
generation of magnetic resonance imaging (MRI) contrast agents, as carriers for
targeted drug delivery, in the hyperthermia and as magnetic separation agent.This
because, first, they have sizes that place them at dimensions comparable to those of a virus (20–500 nm), a protein (5–50 nm) or a gene (2 nm wide and 10–100 nm long). Second, the nanoparticles are magnetic, which means that they obey Coulomb’s law, and can be manipulated by an external magnetic field gradient. Third and finally, nanoparticles have a large surface that can be properly modified to attach biological agents. Applications in biotechnology impose strict requirements on the particles’ physical, chemical and pharmacological properties, including chemical composition, granulometric uniformity, crystal structure, magnetic behavior, surface structure, adsorption properties, solubility and low own toxicity. For example, in order for magnetic drug-targeting to be safe and effective (with the minimum amount of magnetic particles, a maximum of drug should be easily administered and transported to a specific site), the following parameters of the nanomagnets are critical: (a) particle size (small as possible to improve tissular diffusion, and to have long sedimentation times and high effective surface areas), (b) surface characteristics (easy encapsulation of the magnetic nanoparticles protects them from degradation and endows biocompatibility), and (c) good magnetic response (possibility of decreasing nanomagnets concentration in blood and therefore diminishing the associated side effects). Although early research in the
field can be dated back several decades, the recent surge of interest in nanotechnology has significantly expanded the breadth and depth of magnetic nanoparticles research. With a wide range of applications in the detection, diagnosis, and treatment of illnesses,
such as cancer, cardiovascular disease, and neurological disease, Magnetic
nanoparticles may soon play a significant role in meeting the healthcare needs of tomorrow.
4 1.2 Superparamagnetic Nanoparticles
The penetration of magnetic fields through human tissue and the ability to remotely detect or manipulate magnetic materials have been investigated for use in medicine for centuries. To better understand the advantages of using the magnetic nanoparticles in
biomedical field we review some of the fundamental concepts of magnetism and the properties of nanoparticles. More thorough and detailed discussion of this topic can be found in the literature. The classification of a material's magnetic properties is based
on its magnetic susceptibility (χ), which is defined by the ratio of the induced magnetization (M) to the applied magnetic field (H). In diamagnetic materials, the magnetic moment is antiparallel to H resulting in very small and negative
susceptibilities (−10−6 to −10−3). They do not retain magnetic properties when the
external field is removed. Materials with magnetic moments aligned parallel to H and susceptibilities on the order of 10−6 to 10−1 are described as paramagnetic. While in ferri-
and ferromagnetic materials, magnetic moments also align parallel to H, coupling interactions between the electrons of the material result in ordered magnetic states, i.e., magnetic domains, and large spontaneous magnetization. The susceptibilities of these materials depend on their atomic structures, temperature, and the external field H. If we now reduce the size of the ferromagnetic material we may ultimately reach a size where
thermal energy (KBT= 4*10-21 at 300 K) can randomize the magnetization, such that
when there is no externally applied field the magnetization measured in a finite time interval (typically, 100 s) is zero. Such materials, at small sizes (on the order of nanometers), show no coercivity and behave as a single paramagnetic domain with a large magnetic moment, known with the name of superparamagnets (figure 1(a)and (c)). The randomization of the magnetization takes place by excitation over an energy barrier given by the product of the anisotropy constant, K, and the volume, V. Note that the relaxation time, τ, depends exponentially on the energy barrier, KV, and hence to reproducibly control the magnetic behavior of superparamagnetic nanoparticles, narrow size distributions are required (figure 1 (b)). A superparamagnet is defined as an assembly of giant magnetic moments which are not interacting, and which can fluctuate
when the thermal energy, kBT, is larger than the anisotropy energy. However, at
sufficiently high temperatures (i.e., blocking temperature TB) thermal energy is
sufficient to induce free rotation of the particle resulting in a loss of net magnetization in the absence of an external field. This superparamagnetic property, marked by the lack of remanent magnetization after removal of external fields, enables the particles to maintain their colloidal stability and avoid aggregation making it feasible for their use in biomedical applications. Furthermore, the coupling interactions within these single magnetic domains result in much higher magnetic susceptibilities than paramagnetic materials.
Figure 1.Magnetic behavior of materials: ferromagnetic materials (FM) are characterized by exchange interaction, hysteretic behavior and a finite coercivity, Hc, paramagnetic materials (PM) the
non-interacting spins are characterized by a linear susceptibility that is inversely dependent on the temperature (Curie law), superparamagnetic materials (SPM), below a certain critical size the multidomain (FM) becomes a single domain superparamagnetic (a); and the superparamagnetic nanoparticles exhibit no remanence or coercivity, that is, there is no hysteresis in the magnetization curve (c).
Although superparamagnetism is a favorable property of small particles, the reduction of particle size is not without some consequences. As particle sizes decrease, surface-to-volume ratios increase resulting in pronounced surface effects, such as noncollinear spins, spin canting, and spin-glass-like behavior, which can significantly impact the
magnetic properties of the material. Typically, the saturation magnetization (M
values of nanoparticles, corresponding to the complete alignment of all individual (c)
moments in a sample, are smaller than their corresponding bulk phases due to disordered crystal structure resulting from high surface curvature, which increases with particle size reduction. Furthermore, significant differences in magnetic properties are observed with superparamagnetic nanoparticles obtained through different chemical processes. More detailed explanations of the physical properties of superparamagnetic nanoparticles and nanoscale magnetic phenomena can be found in recent reviews.[14,15,16]
The magnetic behaviour of an assembly of nanoparticles is related to the crystalline structure. Among the different nanostructured magnetic materials, the metal oxide, such as magnetite (Fe3O4) and cobalt ferrite (CoFe2O4), with spinel structure (MeIIMe2IIIO4)
represent probably the most promising class in biomedical application, because the rich crystal chemistry of spinels offers excellent opportunities for fine-tuning the magnetic properties. These have a face-centered cubic (fcc) structure in which the oxygen atoms are cubic close-packed. The structure contains two interstitial sites, occupied by metal cations, with tetrahedral, (A)-site, and octahedral, [B]-site, oxygen coordination, resulting in a different local symmetry (figure 2).
Figure 2.Schematic representation of spinel structure.
When the (A)-sites are occupied by MeII cations and the [B]-sites by MeIII cations, the
structure is referred to as normal spinel, (MeII) [MeIII]. However, if the A sites are
completely occupied by MeIII and the B-sites are randomly occupied by MeII and MeIII,
then the structure is referred to as inverse spinel, (MeIII) [MeIII MeII]. In general, the
cationic distribution in octahedral and tetrahedral sites is quantified by the “inversion degree” (γ), which is defined as the fraction of divalent ions in octahedral sites.[17,18]
Tetrahedral site Octahedral site
7 1.3 Synthesis Techniques: Iron Oxide Nanoparticles
It has long been of scientific and technological challenge to synthesize the magnetic nanoparticles of customized size and shape. Physical methods such as gas phase
deposition and electron beam lithography are advantageous in that they produce
nanomaterials of high purity and are applicable to large-scale production, but unfortunately are elaborate procedures that suffer from the inability to control the size
of particles in the nanometer size range. The wet chemical routes to magnetic
nanoparticles are simpler, more tractable and more efficient with appreciable control over size, composition and sometimes even the shape of the nanoparticles.
The most common methods including sol-gel,[21,22] co-precipitation,[23,24] thermal
decomposition,[15,25] hydrothermal synthesis, microemulsion,[27,28] sonochemical
synthesis, and sonochemical synthetic route can all be directed to the synthesis of
high quality of iron oxide nanoparticles. In addition, these magnetic nanoparticles can
also be prepared by the other methods such as electrochemical synthesis,[30,31] laser
pyrolysis techniques. Intable 1 are reported the main synthesis methods used to date
for the preparation of magnetic nanoparticles and the nanoparticle characteristics. Table 1. Comparison of different synthesis methods to produce magnetic nanoparticles
Among these methodologies thermal decomposition and hydrothermal methods seems to lead to the best results in terms of fine particle size tuning and narrow particle size distribution. In order to obtain primary particles of appropriate size and with an adequate distribution of the same, these methods allow to control the kinetically phase nucleation and particle growth through the use of suitable stabilizing agents, often
surfactants. Such stabilizers interact intimately with the surface of nanoparticles, so
that the growth of the nanocrystals is kinetically inhibited by the capping of these
chemical and physical agents. The control of dimensions, of their distribution,
morphology, degree of crystallinity, the agglomeration of particles during and after the synthesis and the manipulation of these materials, constitute critical points for obtaining the final product, given that from these parameters depend on the main properties of nanostructured materials. Recently, the method which has allowed to obtain precise control of size and shape of magnetic nanoparticles with a narrow size distribution, high crystallinity, high stability in organic solvents, is the synthesis based
on the High Temperature Decomposition of organometallic precursors Assisted by
Surfactants (HTDSA). 
Iron oxide nanoparticles with a high level of monodispersity and controlled
size can be obtained by HTDSA of iron organic precursors, such as Fe(Cup)3,
(cup=N-nitrosophenylhydroxylamine), Fe(acac)3, (acac= acetylacetonate), or Fe(CO)5, using
surfactants and high boiling point organic solvents such as the ones shown in table 2. Table 2. High boiling points solvents for thermal decomposition.
By rapidly increasing the reaction temperature to about 200 °C, triggering a burst of nucleation followed by aging at that temperature until the net nucleation rate is zero. Subsequently, the temperature is slowly increased to about the boiling temperature (about 300°C) of the solvent to promote particle growth by diffusion of free atoms to the growing particles. Surfactants such as oleic acid, oleylamine, sodium oleate, and tri-
n-octylphosphine oxide (TOPO) are usually used as coordinating solvent in nucleation phase and growth of nanoparticles, and to avoid particle agglomeration during synthesis. The formation of an intermediate Fe–oleate complex is a critical step in determining the final particle size.[35,36]
1.4 Biomedical applications of Magnetic Nanoparticles
For many biomedical applications, magnetic nanoparticles presenting superparamagnetic behavior (no remanence along with a rapidly changing magnetic state) at room temperature are desirable. Biomedical applications are commonly divided into two major categories: in vivo and in vitro applications. In vivo applications could be
further separated in therapeutic (hyperthermia and drug-targeting) and diagnostic
applications (nuclear magnetic resonance (NMR) imaging), while for in vitro
applications the main use is in diagnostic (separation/selection, and
magnetorelaxometry). Consequently, additional restrictions apply on various
magnetic nanoparticles for in vivo or in vitro biomedical application. It is rather simple for in vitro applications of magnetic nanoparticles. The size restriction as well as
biocompatibility/toxicity are not so critical for in vitro applications, when compared
with in vivo ones. Therefore, superparamagnetic composites containing submicron
diamagnetic matrixes and superparamagnetic nanocrystals can be used. Composites with long sedimentation times in the absence of a magnetic field are also acceptable. It was noticed that functionalities may be provided readily for the superparamagnetic composites because of the diamagnetic matrixes. On the other hand, severe restrictions
all, it is a requisite that the magnetic components should be biocompatible without any toxicity for the biosystems of interest. It is no doubt that interdisciplinary research collaboration is badly needed for clinical and biological applications of magnetic nanoparticles. Research fields involved include chemistry, materials science, cell engineering, clinical tests and other related scientific efforts. In this section, an
overview of the biomedical applications of magnetic nanoparticles will be presented.
Figure 3. Magnetic Nanoparticles in Biomedicine.
1.4.1 Therapeutic applications
Hypertermia.The possibility of treating cancer by artificially induced hyperthermia has led to the development of many different devices designed to heat malignant cells while sparing surrounding healthy tissue. Experimental investigations of the application of
magnetic materials for hyperthermia date back to 1957. Since then there have been
numerous publications describing a variety of schemes using different types of magnetic materials, different field strengths and frequencies and different methods of encapsulation and delivery of the particles. In broad terms, the procedure involves dispersing magnetic particles throughout the target tissue, and then applying an A.C. magnetic field of sufficient strength and frequency to cause the particles to heat. This
heat conducts into the immediately surrounding diseased tissue whereby, if the temperature can be maintained above the therapeutic threshold of 42°C for 30 min or more, the cancer is destroyed. The physical principle for which a magnetic material can be heated by the action of an external alternating magnetic field are the loss processes that occur during the reorientation of the magnetization of magnetic materials with low electrical conductivity. Whereas the majority of hyperthermia devices are restricted
in their utility because of unacceptable coincidental heating of healthy tissue, magnetic particle hyperthermia is appealing because it offers a way of ensuring only the intended target tissue is heated. The advantage of magnetic hyperthermia is that allows the heating to be restricted to the tumour area. Moreover, the use of subdomain magnetic particles (nanometre-sized) is preferred instead multidomain (micron-sized) particles
because nanoparticles absorb much more power at tolerable AC magnetic fields.
Finally, it should be mentioned that the heating potential is strongly dependent on the particle size and shape, and thus having well-defined synthetic routes able to produce uniform particles is essential for a rigorous control in temperature. A number of studies
have demonstrated the therapeutic efficacy of this form of treatment. To date,
however, there have been no reports of the successful application of this technology to the treatment of a human patient. The challenge lies in being able to deliver an adequate quantity of the magnetic particles to generate enough heat in the target using A.C. magnetic field conditions that are clinically acceptable. Most of the laboratory-based studies reported so far are characterised by the use of magnetic field conditions that could not be safely used with a human patient. In most instances, reducing the field strength or frequency to safer levels would almost certainly lead to such a reduction in the heat output from the magnetic material as to render it useless in this application. The frequency and strength of the externally applied A.C. magnetic field used to generate the heating is limited by deleterious physiological responses to high frequency magnetic fields. These include stimulation of peripheral and skeletal muscles, possible cardiac stimulation and arrhythmia, and non-specific inductive heating of tissue. Generally, the usable range of frequencies and amplitudes is considered to be f = 0.05-1.2
MHz and H = 0-15 kAm-1, and a common rule of thumb is that the product H− f should
not exceed 4.85×108 Am-1s-1. The amount of magnetic material required to produce the
required temperatures depends to a large extent on the method of administration. For example, direct injection allows for substantially greater quantities of material to be localised in a tumour than do methods employing intravascular administration or antibody targeting, although the latter two may have other advantages. A reasonable
assumption is that around 5-10 mg of magnetic material concentrated in each cm3 of
tumour tissue is appropriate for magnetic hyperthermia in human patients.
Drug Delivery. The major disadvantage of most chemotherapies is that they are relatively non-specific. The therapeutic drugs are administered intravenously leading to general systemic distribution, resulting in deleterious side-effects as the drug attacks normal, healthy cells in addition to the target tumour cells. For example, the side effects of anti-inflammatory drugs on patients who have chronic arthritis can lead to the discontinuation of their use. However, if such treatments could be localised, e.g. to the site of a joint, then the continued use of these very potent and effective agents could be made possible. Recognition of this led researchers in the late 1970s to propose the use of magnetic carriers to target specific sites (generally cancerous tumours) within the body. The objectives are twofold:
- to reduce the amount of systemic distribution of the cytotoxic drug, thus
reducing the associated side-effects,
- to reduce the dosage required by more efficient, localised targeting of the drug. In magnetically targeted therapy, a cytotoxic drug is attached to a biocompatible magnetic nanoparticle carrier. These drug/carrier complexes usually in the form of a biocompatible ferrofluid are injected into the patient via the circulatory system. When the particles have entered the bloodstream, external, high-gradient magnetic fields are used to concentrate the complex at a specific target site within the body (figure 4).
Figure 4. A hypothetical magnetic drug delivery system shown in cross-section, a magnet is placed outside the body in order that its magnetic field gradient might capture magnetic carriers flowing in the circulatory system.
Once the drug/carrier is concentrated at the target, the drug can be released either via enzymatic activity or changes in physiological conditions such as pH, osmolality, or
temperature, and be taken up by the tumour cells. The process of drug localization
using magnetic delivery systems is based on the competition between forces exerted on the particles by blood compartment, and magnetic forces generated from the magnet, i.e. applied field. When the magnetic forces exceed the linear blood flow rates in arteries (10 cm s-1) or capillaries (0.05 cm s-1), the magnetic particles are retained at the target site
and maybe internalized by the endothelial cells of the target tissue. This system, in theory, has major advantages over the normal, non-targeted methods of cytotoxic drug therapy. The physical principles underlying magnetic targeting therapy are similar to those used in magnetic separation, and are derived from the magnetic force exerted on a superparamagnetic nanoparticle by a magnetic field gradient. The effectiveness of the therapy is dependent on several physical parameters, including the field strength, gradient and volumetric and magnetic properties of the particles. As the carriers (ferrofluids) are normally administered intravenously or intra-arterially, hydrodynamic parameters such as blood flow rate, ferrofluid concentration, infusion route and circulation time also play a major role as do physiological parameters such as tissue depth to the target site (i.e. distance from the magnetic field source), reversibility and strength of the drug/carrier binding, and tumour volume. In general, larger particles
(e.g. magnetic microspheres, around 1 µm in diameter, comprising agglomerates of superparamagnetic particles) are more effective at withstanding flow dynamics within the circulatory system particularly in larger veins and arteries.
Preliminary investigations of the hydrodynamics of drug targeting suggest that for most magnetite-based carriers, flux densities at the target site must be of the order of 0.2 T
with field gradients of approximately 8 Tm-1 for femoral arteries and greater than 100
Tm-1 for carotid arteries. This suggests that targeting is likely to be most effective in regions of slower blood flow, particularly if the target site is closer to the magnet source. As discussed above, there are several major advantages of using magnetic nanoparticles in drug delivery. First, drug bound magnetic nanoparticles can penetrate through small capillaries and be taken up by cells. Secondly, the movement of drug loaded magnetic nanoparticles can be readily controlled by an external magnetic field. Hence, accumulation of efficient drugs at the target sites can be achieved. Thirdly, biocompatible magnetic for example core–shell nanoparticles allow sustained drug release over a period of time. Fourthly, after being injected into bodies, the drug uptake
process can be visualized by MRI.Finally, unlike searching for new molecules, magnetic
drug delivery involves low-cost research, which reduces the cost of drug loaded product. Despite many merits, there are some problems associated with magnetic drug delivery. The major limitation of magnetic drug delivery systems is that the external magnetic field should be lowered to a certain level, higher than which living bodies cannot withstand. However, a magnetic field at this level may not generate magnetic gradient high enough to control the targeted movement of nanoparticles or trigger the drug desorption because the magnetic gradient decreases with the distance. This problem can be alleviated by locating an internal magnet near the target by minimally invasive surgery. Another problem which may occur in magnetic drug delivery is the possible agglomeration of magnetic nanoparticles, that may cause a tough embolization of the blood vessels in the treated area, especially after the removal of the applied magnetic field, due to their high surface energy. Further, smaller nanoparticles possess weaker
magnetic force. Thus, the ultrasmall dimension of nanoparticles, which is required for superparamagnetism, may lead to difficult control of their movement or location in the
presence of a relatively strong drag force from the blood flow. Consequently, magnetic drug delivery is more effectively controlled in blood flows with lower velocities. Further, when applying this technique to human bodies, a magnetic field with a safe strength may not be effective due to the large distance between the target site and the magnet. Pre-clinical and experimental investigations have been carried out to overcome these limitations and improve the efficiency of magnetic drug delivery at a safe level.
1.4.2 Diagnostic applications
The diagnostic applications of magnetic nanoparticles are processes to detect malignant tissues or pathogenic bioaggregates by using magnetic nanoparticles.
MRI contrast enhancement. In life science, an emerging technology, molecular imaging, has been playing a substantial role in both scientific investigation and practical bioapplications. Molecular imaging is the technology that helps us to understand diseases and search for the appropriate treatments. Since most disease processes have a molecular basis, molecular imaging with sufficient image resolution and image contrast at the molecular level is much needed for better diagnostic differentiations, early disease
detection and objective therapy monitoring with imaging biomarkers. There is a
number of molecular imaging techniques available ranging from ultrasonic to gamma ray and X-ray frequencies in the electromagnetic spectrum. Molecular imaging operates at the interface between life science and physical science, and images are obtained by facilitating interaction with a biological entity at a molecular level. Thus, both the life and physical sciences are required to develop and implement a molecular imaging technique due to its diverse nature. Among them, optical imaging, nuclear imaging and magnetic resonance imaging (MRI) are the most widely used molecular imaging techniques. Magnetic nanoparticles are able to enhance the image contrast in MRI, which has attracted enormous attention. To better investigate the functions of magnetic nanoparticles as a contrast agent in MRI, it is necessary to first understand the working mechanism and physical principles in MRI. As far as the imaging mechanism of MRI is
the nuclei of protons are exposed to a strong magnetic field, their spins align either parallel or antiparallel to the magnetic field. During their alignment, the spins precess
under a specified frequency, known as the Larmor frequency (ω0), (figure 5(a)). When a
‘resonance’ frequency in the radio-frequency (RF) range is introduced to the nuclei, the protons absorb energy and are excited to the antiparallel state. After the disappearance
of the RF pulse, the excited nuclei relax to their initial, lower-energy state (figure 5(b)).
There are two different relaxation pathways. The first, called longitudinal or T1
relaxation, involves the decreased net magnetization (Mz) recovering to the initial state
(figure 5(c)). The second, called transverse or T2 relaxation, involves the induced
magnetization on the perpendicular plane (Mxy) disappearing by the dephasing of the
spins (figure 5(d)). Based on their relaxation processes, the contrast agents are classified
as T1 and T2 contrast agents. Commercially available T1 contrast agents are usually
paramagnetic complexes, while T2 contrast agents are based on iron oxide
nanoparticles, which are the most representative nanoparticulate agents.
Figure 5. Principle of magnetic resonance imaging. (a) Spins align parallel or antiparallel to the magnetic field and precess under Lamor frequency (ω0). (b) After induction of RF pulse, magnetization of spins
The reason for using magnetic nanoparticles in MRI is to shorten both T1 and T2* (shorter relaxation time) so that the image contrast can be enhanced. Iron oxide nanoparticles have been tested for contrast enhancement in MRI. Superparamagnetic nanoparticles are magnetically saturated in the common magnetic fields applied in MRI, and they are able to create a substantial locally perturbing dipolar field, and hence successfully decrease the value of T1 and T2*. To further improve biocompatibility, iron oxide-based superparamagnetic nanoparticles are always coated by a biocompatible
layer such as Dextran, PEG, SiO2, DMSA, which can be excreted via the liver after
treatment. In MRI, biofunctionalized magnetic nanoparticles are selectively taken up by the reticuloendothelial system, which serves as a network to remove foreign substances from the blood circulation system. It was found that magnetic nanoparticles with diameter less than 10 nm had a longer half-life than those of 30 nm in diameter or larger in the blood stream. Larger nanoparticles are recognized by liver and spleen, while smaller ones are collected by the reticuloendothelial system in healthy tissues throughout the body. It is the differential uptake of magnetic nanoparticles by different tissues that determines the MRI contrast. For tumor cells, the relaxation times are not changed by introducing contrast agent (magnetic nanoparticles) due to the absence of an effective reticuloendothelial system in the tumor. Therefore, identification of malignant lymph nodes, liver tumors and brain tumors by comparing the image contrast can be readily achieved in the presence of magnetic nanoparticles in MRI. It has been also noticed that iron oxide nanoparticles have the capability of being encapsulated into target-specific agents. Another type of common contrast agents T1 used in MRI is paramagnetic gadolinium ion complexes. Generally, magnetic labeling is employed by using fluorescent-labeled magnetic nanoparticles in both in vitro and in vivo imaging. The combination of nanoscale dimensions, superparamagnetic properties and fluorescence for these bifunctional nanoparticles has prompted their use in medical imaging which combines fluorescent imaging techniques and the MRI approach. Both methods are of great importance in diagnostic and therapeutic applications because cellular monitoring provides valuable information for subsequent cell-based therapy. The advantage of the MRI technique is well known: it offers anatomically sensitive deep
tissue imaging. As discussed above, magnetic resonance imaging is one of the most powerful medical tools for diagnostic purposes owing to its noninvasive process, high spatial resolution and multidimensional tomographic capabilities. However, this technique suffers from low-signal sensitivity. To overcome the weakness of current MRI techniques, signal enhancers need to be used. The signal-enhancing capabilities of
magnetic nanoparticles/nanocrystals have been demonstrated. Magnetite (Fe3O4), as a
member of clinically benign iron oxide-based nanoparticles, has been widely explored for signal-enhancing purposes.
Magnetic Separation and Purification. In modern biology or biomedicine, separation of particular biological entities (e.g. DNA, proteins, ions, molecules, etc.) from their native environment is often required for both scientific investigation and practical uses. Magnetically labeled biological entities exhibit magnetic properties so that they can be separated by applying an external magnetic field. Due to this reason, magnetic separation and purification have been widely used to prepare concentrated bio-samples in biomedical applications. A typical magnetic separation usually contains two steps: labeling desired biological entities with magnetic materials and separating magnetically tagged entities via a magnetic separation device. To ensure an effective labeling, functionalization needs to be performed to deposit biocompatible molecules on magnetic nanoparticles. The organic or inorganic coating not only provides a link between the particles and target biological entities, but improves the colloidal stability. A highly effective method of labelling cells is via antibody/antigen bonding due to its specific binding characteristics. By this technique, various biological entities (e.g. cancer cells, bacteria, red blood cells, Golgi vesicles, etc) have been demonstrated binding to immunospecific agents–coated magnetic nanoparticles. Similarly, magnetic microparticles can also be used for larger entities when incorporated in a polymer binder. In the second step of magnetic separation, when the mixture passes through a magnetic field, magnetic labeled targeted materials immobilize because of the force due
to the magnetic field gradient and separate from the native solution. Due to the
achieved by simply using a permanent magnet to aggregate magnetic entities on the wall of a test tube followed by removal of the supernatant. This simple process is illustrated
in figure 6(a).
Figure 6. Schematic of two standard methods for magnetic separation. (a) A magnet is placed close to the container wall of a solution containing magnetically tagged (•) and unwanted (◦) biomaterials. Due to the magnetic force exerted the tagged particles are attracted by the magnet and agglomerate while the unwanted biomaterials can be removed with the supernatant solution; (b) a solution containing tagged and unwanted biomaterials flows continuously through a region with strong magnetic field gradient which can be provided by packing the column with steel wool. Thus the tagged particles can be attracted. Afterwards, the tagged particles can be collected after removing the field followed by flushing through with water.
However, this method is suffering from its low separation efficiency because of the slow accumulation rates. Thus better magnetic separation is needed. A common method of achieving high separation efficiency is to use a magnetizable matrix of wire or beads to apply a strong magnetic field on a flow column through which magnetically tagged fluid is pumped. The type of separator design is able to generate high magnetic field gradient and capture the magnetic biological entities efficiently as they flow with their carrier
medium. Figure 6(b) depicts the schematic of this process. In spite of its faster
separation, this method, however, has some problems caused by the settling and adsorption of magnetic materials on the matrix. To overcome this problem, an alternative separation design was developed, as shown in figure 7.
20 Figure 7. Schematic illustration of a rapid throughput method for magnetic separation. In this method, a solution containing magnetically tagged (•) and unwanted (◦) biomaterials flows through an annular column placed within a set of magnets arranged in quadrature. (a) Longitudinal cross-section view of the annular column showing the flow of the solution; (b) transverse cross-section view of the four magnets with the resulting magnetic field lines. Under the magnetic force due to the magnetic field gradient, the tagged particles are attracted to the column walls, where they are held until the field is removed. The held tagged biomolecules can be recovered by flushing the column with water.
In this design, a magnetic gradient is created radially outwards from the center of the flow column by a quadrupolar arrangement. So obstruction will not take place during the separation. Additionally, biological entities with different magnetophoretic mobilities can be fractioned to achieve ‘fluid flow fractionation’ by adjusting the magnitude of the field gradient. In a typical separation process, the applied magnetic field is moved up the column while the fluid is kept static. Consequently, the particles can be moved up by the magnetic force and collected by a permanent magnet. The bottom section of fluid is then subjected to repeat separation processes with different magnetic strengths. Magnetic separation can be used with optical sensing to perform ‘magnetic enzyme linked immunosorbent assays’. Immuno-assays, combined with fluorescent enzymes, are able to detect cells labeled by the enzymes. In contrast to a conventional means in which the target cells need to bind to a solid matrix, magnetic-assisted immunosorbent assays utilize magnetic microspheres as the surface for cell immobilization. Importantly, magnetic separation is typically used to increase the concentration of the target materials. Recently, magnetic nanoparticles have been employed in this assay application. The use of nanoparticles improves the magnetic separation efficiency because their high mobility results in a short reaction time and
more immobilized reagent. Furthermore, magnetic separation offers an effective way to localize labeled cells at certain locations, which is of great help for cell detection and number counting by optical scanning.[3, 38]
 B.L. Cusching, V.L. Kolesnichenko, C.J. O’Connor, Recent Advances in the Liquid-Phase Syntheses of Inorganic Nanoparticles. Chem. Rev. 2004, 104, 3893-3946.
 C. Corit, P. Robert, J.M. Idee, M, Port, Recent advances in iron oxide nanocrystal technology for medical imaging. Advaced Drug Delivery Reviews, 2006, 58, 1471-1504.
 Q.A. Panknurst, J. Connolly, S.K. Jones, J. Dobson, Applications of magnetic nanoparticles in biomedicine. Journal of Physics. D, Applied Physics, 2003, 36, 167-181.
 P. Pradhan, J. Giri, R. Banerjee, J. Bellare, D. Bahadur, Preparation and characterizations of manganese ferrite based magnetic liposomes for hyperthermia treatment of cancer. J. Magn. Magn.
Mater., 2007, 311, 208-215.
 Q.A. Pankhurst, Nanomagnetic medical sensors and treatment methodologies. BT Technology
Journal, 2006, 24, 33-38.
 P. Tartaj, M.P. Morales, T. Gonzàles-Carreño, S. Veintemillas-Verdaguer, C.J. Serna,
Advances in magnetic nanoparticles for biotechnology applications. Journal of Magnetism and
Magnetic Materials, 2005, 28-34.
 M. Ferrari, Cancer nanotechnology: opportunities and challenges. Nature Reviews, Cancer,
2005, 5, 161-171.
 S.A. Wickline, A.M. Neubauer, P.M. Winter, S.D. Caruthers, G.M. Lanza, Molecular
imaging and therapy of atherosclerosis with targeted nanoparticles. Journal of magnetic Resonance
Imaging, 2007, 25, 667-680.
 C. Corot, K.G. Petry, R. Trivedi, A. Saleh, C. Jonkmanns, J.F. Le Bas, E. Blezer,
M.Rausch, B. Brochet, P. Foster-Gareau, D. Baleriaux, S. Gaillard,V.Dousset, Macrophage
imaging in central nervous system and in carotid atherosclerotic plaque using ultrasmall superparamagnetic iron oxide inmagnetic resonance imaging. Investigative Radiology, 2004, 39, 619-625.
 C. Sun, J. S.H. Lee, M. Zhang, Magnetic nanoparticles in MR imaging and drug delivery.
 M.R. Mourino, From Thales to Lauterbur, or from the lodestone to MR imaging: magnetism and medicine. Radiology, 1991, 180, 593-612.
 A. Morrish, The Physical Principles of Magnetism. IEEE Press, New York, 2001.
 A.H. Lu, E.L. Salabas, F. Schuth, Magnetic nanoparticles: synthesis, protection,
functionalization, and application. Angewandte Chemie. International Edition, 2007, 46,
 X.M. Lin, A.C.S. Samia, Synthesis, assembly and physical properties of magnetic nanoparticles.
Journal of Magnetism and Magnetic Materials, 2006, 305, 100-109.
 C. Cannas, A. Musinu, A. Ardu, F. Orrù, D. Peddis, M. Casu, R. Sanna, F. Angius, G. Diaz, G. Piccaluga, CoFe2O4 and CoFe2O4/SiO2 Core/Shell Nanoparticles: Magnetic and
Spectroscopic Study. Chem. Mater., 2010, 22, 11, 3353-3361.
 D. Peddis, F. Orrù, A. Ardu, C. Cannas, A. Musinu, G. Piccaluga, Interparticle
Interactions and Magnetic Anisotropy in Cobalt Ferrite Nanoparticles: Influence of Molecular Coating.
Chem. Mater., 2012, 24, 6, 1062-1071.
 A.R. West, Solid State Chemistry and its Applications, Series, 1984.
 L. Suber, D. Peddis, Approaches to Synthesis and Characterization of Spherical and Anisometric metal Oxide Magnetic Nanoparticles. Nanomaterials for the Life Sciences Vol.4:
Magnetic Nanomaterials, Wiley-VCH, 2009.
 S. Stolnik, L. Illum, SS. Davis, Long circulating microparticulate drug carriers. Adv. Drug
Del. Rev., 1995, 16, 195-214.
 A.K. Gupta, S. Wells, Surface modified superparamagnetic nanoparticles for drug delivery: preparation, characterization and cytotoxicity studies. IEEE Trans Nanobiescience, 2004, 3, 1,
 C.J. Brinker, Sol-Gel Science. Academic Press, San Diego, 1990.
 C. Cannas, A. Falqui, A. Musinu, G. Piccaluga, D. Gatteschi, C. Sangregorio, G. Concas, G. Spano, Superparamag netic behaviour of γ-Fe2O3 nanoparticles dispersed in a silica
matrix. Chem. Phys., 2001, 3, 832-838.
 A.K. Gupta, M. Gupta, Synthesis and surface engineering of iorn oxide nanoparticles for biomedical applications. Biomaterials, 2005, 26, 3995-4021.
 S. Sun, H. Zeng, D.B. Robinson, S. Raoux, P.M. Rice, S.X. Wang, G. Li, Monodisperse MFe2O4 (M= Fe, Co, Mn) Nanoparticles. J. Am. Chem. Soc., 2004, 126, 273-279.
 X. Hu, J.C. Yu, J. Gong, Fast production of self-assembled hierarchical- Fe2O3
nanoarchitectures. J. Phys. Chem. C, 2007, 111, 11180-11185.
 C. Solans, P. Izquierdo, J. Nolla, N. Azemar, M.J. Garcia-Celma, Nano-emulsions. Curr.
Opin. Colloid Interface Sci., 2005, 10, 102-110.
 C. Cannas, A. Ardu, D. Peddis, C. Sangregorio, G. Piccaluga, A. Musinu,
Surfctant-assisted route to fabricate CoFe2O4 individual nanoparticles and spherical assemblies. Journal of Colloid and Interface, 2010, 343, 415-422.
 J.H. Bang, K.S. Suslick, Sonochemical Synthesis of Nanosized Hollow Hematite. J. Am.
Chem. Soc., 2007, 129, 2242-2243.
 L. Cabrera, S. Gutierrez, N. Menendezb, M.P. Morales, P. Herrasti, Magnetite
nanoparticles: Electrochemical synthesis and characterization. Electrochim. Acta, 2008, 53,
 C. Pascal, J.L. Pascal, F. Favier, M.L.E. Moubtassim, C. Payen, Electrochemical synthesis for the control of gamma-Fe2O3 nanoparticles size. Morphology, microstructure, and magnetic behavior. Chem. Mater., 1999, 11, 1, 141-147.
 O. Bomatì-Miguel, L. Mazeina, A. Navrotsky, S. Veintemillas-Verdaguer, Calorimetric Study of Maghemite Nanoparticles Synthesized by Laser-induced Pyrolysis. Chem. Mater., 2008,
20. 2, 591-598.
 N.A. Kotov, I. Dekany, J.H. Fendler, Layer-by-layer self assembly of polyelctrolyte-semiconductor nanoparticle composite films. J. Phys. Chem., 1995, 99, 13065-13069.
 J. Park, J. Joo, S.G. Kwon, Y. Jang, T. Hyeon, Synthesis of monodisperse spherical
nanocrystals. Angewandte Chemie, 2007, 46, 4630-4660.
 N.R. Jana, Y. Chen, X. Peng, Size and shape-controlled magnetic ( Cr, Mn, Fe, Co, Ni) oxide nanocrystals via a simple and general approach. Chem. Mater., 2004, 16, 3931-3935.
 A.G. Roca, R. Costo, A.F. Rebolledo, S. Veintemillas-Verdaguer, P. Tartaj, T.
Gonzàlez-Carreño, M.P. Morales, C.J. Serna, Progress in the preparation of magnetic
nanoparticles for applications in biomedicine. J. Phys. D: Appl. Phys., 2009, 42, 1-11.
 P. Tartaj, M. del Puerto Morales, S. Veintemillas-Verdaguer, T. Gonzàlez-Carreño, C. J Serna, The preparation of magnetic nanoparticles for applications in biomedicine. J. Phys. D:
Appl. Phys., 2003, 36, 182-197.
 V. K. Varadan, L.F. Chen, J. Xie, Nanomedicine: Design and Applications of Magnetic Nanomaterials, Nanosensors and Nanosystem. John Wiley & Sons, 2008, 1-484.
 M.A. El-Sayed, Some Interesting Properties of Metals Confined in Time and Nanometer Space of Different Shapes. Acc. Chem. Res., 2001, 257-264.
 R. Hiergeist, W. Andra, N. Buske, R. Hergt, I. Hilger, U. Richter, W. Kaiser,
Application of magnetite ferrofluids for hyperthermia. J. Magn. Magn. Mater., 1999, 201,
 A. Jordan, R. Scholz, P. Wust, H. Fähling, R. Felix, Magnetic fluid hyperthermia (MFH): Cancer treatment with AC magnetic field induced excitation of biocompatible superparamagnetic nanoparticles. Journal of Magnetism and Magnetic Materials, 1999, 201, 413-419.
 P. Moroz, S.K. Jones, B.N. Gray, Magnetically mediated hyperthermia: current status and future directions. International Journal of Hyperthermia, 2002, 18, 267-284.
 W.J. Atkinson, I.A. Brezovich, D.P. Chakraborty, Usable Frequencies in Hyperthermia with Thermal Seeds. IEEE T Bio-Med Eng., 1984, 31, 70-75.
 J.C. Joubert, Magnetic Microcomposites as Vectors for Bioactive. Agents: The State of Art. An.
Quim. Int. Ed., 1997, 93, 70-76.
 A.S. Lübbe, C. Bergemann, J. Brock, D.G. McClure, Physiological aspects in magnetic drug-targeting. J. Magnetism and Magnetic Materials, 1999, 194, 149-155.
 M. Arruebo, R. Fernandez-Pacheco, M.R. Ibarra, J. Santamaria, Review: Magnetic
nanoparticles for drug delivery. Nanotoday, 2007, 2, 22-32.
 P.J. Cassidy, G.K. Radda, Molecular imaging perspectives. J. Roy Soc. Interface, 2005, 2,
 H. Bin Na, I.C. Song, T. Hyeon, Inorganic Nanoparticles for MRI Contrast Agents. Adv.
Surface Modification and Silica Nanocomposite
Superparamagnetic nanoparticles have been widely used for numerous in vitro and in vivo applications. All these biomediacal and bioengineering applications require that these nanoparticles need special surface coating of the magnetic nanoparticles, which has to be not only non-toxic and biocompatible but also allow a targetable delivery with particle localization in a specific area. This chapter focuses on the surface modification of the magnetic nanoparticles through organic and inorganic coatings. The type of specific coating depends on the end application and should be chosen by keeping a particular application in mind.
Surface Modification and Silica Nanocomposite
2.0 Surface modification of magnetic nanoparticles 2.1 Introduction
Superparamagnetic iron oxide nanoparticles with appropriate surface chemistry have been widely used experimentally in biomedical field. The biomedical and bioengineering applications require that these nanoparticles have high magnetization values and size smaller than 100 nm with overall narrow particle size distribution, so that the particles have uniform physical and chemical properties. In addition to these applications, the
development of methods aimed at the post-synthetic surface modification of magnetic nanoparticles is important to render them not only non-toxic, biocompatible, soluble in water, but chemically functional, and thus allow a targetable delivery with particle localization in a specific area. Several magnetic oxides have been synthesized using water-based methods like coprecipitation, oil in water microemulsions or micelles strategies, hydrothermal and sonochemistry processes.[2,3,4,5,6] The disadvantage of these aqueous solution syntheses is that the nanoparticle quality, more specifically their size and shape uniformity and in some cases crystallinity, is rather poor. About ten year ago, a new synthetic procedures have been developed to obtain scalable preparative routes
for high-quality magnetic nanoparticles, that could be synthesized by thermal
decomposition of different types of iron precursors such as iron acetylacetonate,[8,9] iron
pentacarbonyl, and iron-oleate, in the presence of surfactants, such as oleic acid and
oleylamine. The nanoparticles resulting from this procedure are stable in nonpolar solvents (such as hexane or cyclohexane) and capped with nonpolar end-groups on their surface. The capping molecules (also called ligands) are typically long-chain alkanes with polar groups that bind to the nanoparticles’ surface. Although the thermal decomposition method has the advantage of producing very monodisperse particles, it has the big disadvantage that the resulting nanoparticles are only dispersible in nonpolar solvents, which to some extent limits their applications in biological fields. Hence, to make ferrite magnetic nanoparticles suitable for biological applications, the hydrophobic surfactant coating needs to be replaced by a hydrophilic, biocompatible, and functional coating that allows controlled interaction with biological species. In literature recently lot of work has been made in this direction; hydrophobic magnetic nanoparticles have been coated with organic or inorganic systems. [9,12-14]
2.2 Surface modification
The colloidal stabilization of the magnetic nanoparticles in both aqueous and physiological medium is crucial for their therapeutic applications and can be achieved by either charging the surface or conjugating it by macromolecules for steric hindrance. The surface charge can be monitored and ensured by suitable means such as changing pH of the medium or modifying with functional groups. The steric stabilization can be achieved by attaching/grafting of organic small molecules, macromolecules, and inorganic coating on the surface. The steric stabilization is indeed less sensitive to the ionic strength of the suspension medium and can be easily achieved in both polar and non-polar medium. The oxide nanoparticles may be stabilized either during their synthesis or in a post-synthesis process. The in situ modification during synthesis process has several advantages including reduced agglomeration.
30 2.2.1 Organic coating
The binding affinity of large surfactant molecules or long polymer chains to the nanoparticles may be lost due steric hindrances, which could otherwise be easily overcome by using small molecules having multiple functional groups such as carboxyl
(COOH), amine (NH2), thiol (SH), phosphate and sulfates. These stabilizers can be
tailored for dispersibility into aqueous media or other biocompatible fluids. The presence of hydroxyl groups on the surface of oxide nanoparticles provides a versatile route for multiple functionalities. Furthermore, the presence of large number of functional groups on the surface of nanoparticles may be used for linkage of various
biomolecules as well as drugs. Among various small molecules, citrate moiety having
multiple carboxylate functionalities, aminesilane for amine groups used as stabilizing
agent, and dimercaptosuccinic acid (DMSA), because having thiol functionality achieved
great deal of attention due to their higher binding affinity towards metal and metal oxide nanoparticles.
Macromolecules.A variety of polymer molecules have been used for steric stabilization
of oxide nanoparticles in aqueous and high ionic strength media. The polymer shell
improves the stability of nanoparticles in solution and allows the encapsulation of a therapeutic agent. Further, these stabilizers provide a means to tailor the surface properties of nanoparticles such as surface charge and chemical functionality or their thermosensitive properties. Major facts with regard to polymeric stabilizer that may affect the performance of nanocarriers include the chemical nature of the polymer (i.e., hydrophilicity/hydrophobiciy, biocompatibility and biodegradation), the molecular weight of the polymer, the manner in which the polymer is grafted or attached (i.e., physically or chemically), the conformation of the polymer and the degree of particle
surface coverage. Among various macromolecules, dextran has been widely used for
surface modification mostly because of its favorable size (chain length) and biocompatibility, which enables optimum polar interactions (mainly chelation and hydrogen bonding). Dextran coating not only provides a smooth outline and narrow size distribution but also retains the essential superparamagnetic behavior of iron oxide
nanoparticles and a significantly prolonged the storage stability.PEG is hydrophilic,
water-soluble, biocompatible polymer and extensively used to increase blood circulation times.
Other coating. The amphiphilic molecules such as liposomes have been successfully used
to stabilize oxide nanoparticles for therapeutic application. Liposomes have also the
ability to encapsulate a large number of nanoparticles and deliver them together to the specific target site. Both hydrophilic and hydrophobic foreign molecules such as drugs and biomolecules can be easily anchored to the amphiphilic liposomes which can enhance the multifunctionality of a system.
2.2.2 Mechanisms of surface modification by organic molecules
Ligand exchange. This is a an alternative method for tuning the surface properties of nanoparticles. The concept of ligand exchange is very simple: mixing nanoparticles wit the free ligands results in replacement of outgoing ligands with the incoming ones.
Exchanging weakly bound ligands for strongly binding ligands is to replace a strongly bound ligand with a ligand present in high concentration during the exchange procedure. This drives the equilibrium towards the thermodynamically less stable nanoparticles (NP) coated with weakly binding ligands; thus satisfying Le Chatellier’s principle:
][ ]n m m n X X NP Y X NP K − − =
where n and m are the number of molecules of X and Y respectively.
The position of this equilibrium depends on the properties of the incoming and outgoing ligand. If the ligands have similar structure, the equilibrium constant is close to 1. For
functionalized ligands, however, the situation becomes much more complicated. The true equilibrium may be difficult to achieve as there are some very slow processes on the nanoparticle surface which do not go to completion even after many days. These processes can disturb the apparent equilibrium position. The exact number of ligands
per nanoparticle is often unknown, and not all ligands can be exchanged; this makes accurate determination of the equilibrium constant difficult. Additionally, the position of equilibrium seems to depend on the exact ratio of incoming to outgoing ligands, presumably due to the different reactivity of different binding sites on the nanoparticles surface. The main advantages of the method are the simplicity and the fact that the
process not increase the size of the nanoparticles due to the small size of the exchange
agents such as silanes, tetramethylammonium hydroxide, silsesquioxane,
carboxylic, phosphonic, mercaptoalkanoic acids, and polymers. However, this
method relies on the exchange of the surfactant coating ligands with the substitutional molecule of which one end carrying a functional group that is reactive toward the nanocrystal surface and the other end carrying a hydrophilic group as carboxylic or sulfonic acid , that are found to stabilize the particles for longer time. Due to the
relatively high prevalence of potential ligands in vivo, including thiols, carboxylic acids,
peptides, sugars and phosphates; ligands on nanoparticles intended for in vivo use must
have a high enough affinity for the nanoparticles that they will not undergo significant exchange with these species. The stability of ligand shells is governed by many of the same factors that stabilize self-assembled monolayers. Stability is dominated by the strength of the ligand-surface bond, but the ability of the ligand tails to pack in an ordered fashion is also significant. The structure and hence the stability of a ligand shell can be altered by the position of a single methyl group, the presence or absence of a
single unsaturated bond or other packing factors such as chain length and π-π
stacking. The concentration of free ligands available to form a monolayer also
influences the ligand orientation and hence degree of stabilization afforded. Light
induced reactions at the nanocrystals/ligand interface can also often lead to desorption of the ligands.[25,40] In aqueous solution, the ligand-nanoparticle interaction is basically
the same but a number of different effects important for stability arise. Most commonly, hydrophilic nanoparticles are stabilized by electrostatic repulsion by the equally charged ligand molecules on the particle surface. However, in the presence of high salt concentration the electric field is shielded and the nanoparticles can come close to each other until eventually attractive forces cause the particles to agglomerate, as induced